Bogusawska-Bczek M, Hes L. Effective Water Vapour Permeability of Wet Wool Fabric and Blended Fabrics.FIBRES & TEXTILES in Eastern Europe 2013; 21, 1(97): 67-71.
Effective Water Vapour Permeability of Wet Wool Fabric and Blended Fabrics
Monika Bogusawska-Bczek, *Lubos Hes
University of Bielsko-Biala, Faculty of Materials and Environmental Sciences,
Institute of Textile Engineering and Polymers Materials,
Department of Textile Engineering and Science of Commodities,
ul. Willowa 2, 43-309 Bielsko Biaa, Poland, E-mail: email@example.com
*Technical University of Liberec, Faculty of Textile Engineering,
Department of Textile Evaluation, Liberec, Czech Republic
AbstractThe water vapour permeability of fabrics is one of the most important factors determining wearer comfort. Contrary to commonly accepted theories, outerwear is often used in a wet state, which has an influence on their properties. However, common standard measuring instruments mostly do not enable reliable measurement of wet fabrics due to the long time of measurement, during which the fabrics get dry. This paper presents the fast instrument - Permetest, which provides reliable measurement of the water vapour permeability of fab-rics in a dry and wet state. By means of the instrument, the relative and effective water vapour permeability of different wool fabrics in a dry and wet state were determined and the results discussed. The main contribution of the measurement was the determination of the exact ratio between the level of heat flux density of the heat flow penetrating the wet fabric, having a cooling effect, and that of the heat flux density of the heat flow caused by moisture evaporation from the fabric surface, also having a cooling effect.
Key words: water vapour permeability, Permetest, wet fabrics, cooling, heat flow.
wet state, a water film on the outer fabric surface is formed, which may reduce the effective permeability of the fabric [6, 7]. Meanwhile wet skin can greatly in-crease the cooling effect of the body, and hence, for example, a moisture content of 10 - 20% could cause a drop in thermal insulation of up to 50% compared to the dry fabric. Sweat production by the hu-man body depends on the type and in-tensity of physical activity, and changes from 40 100 g/h (standard perspiration) to even up to 1 litre of sweat in an hour (very heavy physical work). Therefore it seems very important to investigate the water vapour permeability of fabric not only in a dry state but also in a wet state, which applies in particular to fabrics with high hygroscopicity, which wool fabrics have. Unfortunately, the permeabil-ity cannot be detected by common WVP testers because the samples during this measurement get dry as a result of too long time of measurement. The only in-struments that are suitable for WVP eval-uation of wet fabrics are instruments of the Skin Model Type (f.e. PERMETEST Sensora Skin Model), which allow to perform tests quickly and reliably .
n Theoretical assumptionsThe heat flux density generated due to sweat evaporation determines heat lost by the body and has a cooling effect on it. The heat flux density also has an ef-fect on cooling due to the moisture which evaporates from the surface of the fabric (see Figure 1, page 68). However, this cooling effect may not cool the body suf-ficiently because the heat flux density caused by the temperature drop at the fabric surface is reduced by the effect of
tair - gradient of ambient temperature qs - heat flux passing through the meas-uring head covered by the sample, W.m-2,
U - relative mass increase of the fabric with moisture content in %, determined by weighing,
h - thickness of air gaps between the meas-uring surface and fabric, m,
k experimentally determined constant characterising the decrease in thermal resistance caused by the increased moisture U of the fabric.
n IntroductionThermal comfort implies the main-tenance of body temperature within relatively narrow limits. Under condi-tions where thermal comfort cannot be achieved by the human bodys own abil-ity (i.e. body temperature regulation), such as very cold or hot weather, clothing must be worn to support its temperature regulation by resisting or facilitating heat exchange between the human body and the environment. Together with good in-sulation, the garment should allow ad-equate transport of water vapour from the body to the external environment. Thus the final thermo-physiological comfort is given by two principal components: ther-mal resistance in a wet state and active cooling resulting from moisture evapora-tion from the skin and passing through the garment and from direct evaporation of sweat from the fabric surface [1, 2]. Fundamental papers on fabric thermal resistance and water vapour permeability have been published [3 - 5], but they did not take into consideration the aspect of changes in these parameters due to the moisture content of fabrics. In a dry state, most fabrics deliver satisfactorily perme-ability to water vapour (WVP), but in a
Survey of symbols used, - convection heat, W.m-2K-1,p - mass transfer coefficients,
kg.m-2Pa-1s-1,L - latent heat of evaporation of water,
J kg-1, qfabw - density of heat flux caused by con-
vection mass transfer from the fabric surface, W.m-2,
qfabw,sk - density of heat flux causing skin cooling by evaporation from the wet fabric, W.m-2,
qskin - density of heat flux evaporated from the skin, W.m-2,
qtot - density of heat flux (qtot) transferred through the boundary layer on the fabric surface, W.m-2,
qo- density of heat flux passing through the uncovered measuring head, W.m-2,
psat, psat,fab - saturated water vapour pres-sure on the skin and fabric surface in Pa, which increases with the skin and / or fabric temperature,
pwo - water vapour saturate partial pres-sure valid for the temperature of air in the measuring laboratory, Pa,
pair - water vapour pressure of outside air, Pa,
Reto, Rcgap - evaporative resistance of the boundary layer and air gap, Pa.m2W-1,
Ret evaporative resistance of the fabric, Pa.m2W-1,
Rct, Rgap - thermal resistances of the fabric in an ultra-dry state and that of the air gap, K.m2W-1,
Rctw - thermal resistance of the fabric in a wet state, Km2W-1,
Dp - diffusion coefficient related to water vapour partial pressure and heat flow, W/Pa.m,
FIBRES & TEXTILES in Eastern Europe 2013, Vol. 21, No. 1 (97)68
thermal resistance of the fabric and by that of the air gap between the fabric and skin [9, 10]. In this study the effect of the contact thermal resistance is neglected. Figure 2 shows all the evaporation re-sistances Ret in Pa.m2/W encountered during the passage of heat flux density caused by the evaporation of sweat to the environment.
At first, the effect of skin cooling caused by the evaporation of moisture from the fabric surface was analysed. Despite the assumption of isothermal conditions, the wet fabric becomes cooler than the sur-rounding air because the fabric surface, due to the effect of a certain fabric ther-mal resistance, is not kept at the tempera-ture of the instruments (Skin Model) measuring surface. The heat flux density, caused by convection mass transfer from the fabric surface (qfabw), can be de-scribed by Equation 1, on condition that the fabric surface is covered by a contin-uous water film :
qfabw = L p(psat, fab pair) (1)
The force which causes water vapour transfer can be expressed as the differ-
Equation 5 confirms that with increasing fabric moisture, fabric thermal resistance decreases, which causes an increase in the cooling effect by conducting the heat flux away from the skin. This explanation can be simplified - the increase in moisture of the fabric will also probably be fol-lowed by an increase in the mass transfer area, at least to some extent. The heat flux density evaporated from the skin (qskin) can be then described by Equation 6, provided that the partial pressure of wa-ter vapour at the skin surface reaches the saturated level (this assumption is used by many researchers [1, 6]):
The evaporative resistance of the rela-tively narrow air layer (Rgap) without the contribution of free convection  can be described as:
Rgap = h/Dp (7)
The evaporative resistance of the bound-ary layer (Reto) yields the next equation:
Reto = 1/ p (8)
Thus the flux density of the total heat flux (qtot) transferred through the bound-ary layer on the fabric surface is obtained (with some simplifying assumptions like neglecting the heat transfer by radiation) from the sum of heat flux densities of heat flux passing from the skin through the permeable fabric and the heat flux caused by the temperature gradient between the skin and fabric surface, which is cooled
ence in partial pressures of water vapour, or as the difference in water vapour con-centrations. In the Ergonomic Sciences, the use of partial pressures of water va-pour (Equation 1) is more common [1, 6]. Except for dry and very dry fabric states, a continuous water film is present at any level of fabric moisture - it is called the period of constant drying velocity and constant fabric surface temperature. Dur-ing this period, the partial pressure of wa-ter vapour at the skin surface reaches sat-uration. The heat flux density qfabw must be in equilibrium with thermal losses by convection to the outside air and heat conduction towards the skin:
L p (psat,fab - pair) == tair + tair /(Rctw + Rgap)
The thermal resistance of the fabric in a wet state Rctw can be in the first appr